effect of crumb rubber modifiers (crm) on performance-relatedra- 2015-12-04آ effect of crumb...
Post on 30-Mar-2020
Embed Size (px)
1Research Associate and Assistant Professor of CEE and 2Graduate Research Assistant, The Pennsylvania Transportation Institute, The Pennsylvania State University, University Park PA The oral presentation was made by Professor Bahia
Effect of Crumb Rubber Modifiers (CRM) on Performance-Related Properties of Asphalt Binders
Hussain U. Bahia1 and Robert Davies2
Introduction Crumb rubber derived from used vehicular tires has been used for a wide variety of industrial applications (1).
In the early 1960's, pavement engineers in the United States started experimenting with the use of crumb rubber as a modifier to asphalt cement used in pavement applications (2). Different approaches were used to incorporate crumb rubber modifier (CRM) in road paving materials. In general these approaches are at the present time classified as the dry method and the wet method (3). The wet method involves dispersing the CRM particles into the asphalt cement to produce what is called asphalt rubber (AR) which in turn is used to produce hot-mix asphalt concrete. The dry process involves mixing the CRM with the aggregate before introducing the asphalt cement to the mixture.
Although the use of asphalt rubbers for paving applications is not new, and although there are now a number of paving contractors specialized in AR, only a few studies have been reported on how these binders differ from unmodified binders in general, and how the rubber particles change the properties of the base asphalt cements used in their production (4,5,6,7,8). Furthermore, these few reports were for the most part based on conventional types of binder testing with limited scopes. The asphalt rubber industry is now expanding, in particular following the mandate of recycling used tires included in the Intermodal Surface Transportation Efficiency Act (ISTEA) of 1991. The mandate in many ways created a significant dispute about the usefulness of using CRM in asphalt pavements, about whether there are enough data to support the technical soundness of the mandate, and about what is the most efficient approach to satisfy the mandate.
The one point upon which all parties involved are in agreement is the fact that scientific research on the effect of CRM on asphalt binder properties is sparse, and that there are no established procedures for the successful use of CRM in the asphalt pavement industry. This fact has resulted in a confusion on the part of the pavement industry and State agencies as to what type of CRM to use, how to use it, how to construct it, and whether or not the added cost is justified. In November of 1990 there were more than 30 producers of CRM and the number since then is increasing rapidly. Production of CRM can vary significantly and can result in CRM that will affect the asphalt binder or mixtures in a vastly different manner. The few studies reported about CRM have already shown that method by which CRM is produced is of significant consequences on the properties of asphalt rubbers (6). There are now emerging technologies by which CRM properties can be altered or customized to meet application- specific requirements. There are additives that are being introduced to CRM asphalts to better their performance.
The purpose of this paper is to summarize the results of the first phase of a project to evaluate the effect of CRMs produced by different processes on basic rheological, failure, and aging properties of asphalt binders. The evaluation was done using the new testing and aging procedures developed for the Strategic Highway Research Program. Three common types of CRM and four asphalts selected with different compostional properties were used in the testing program. Measurements included rheological properties across a wide range of temperatures covered in the Performance Grade (PG) specification introduced by SHRP. The rotational viscometer was used to measure response at pumping, storage, and construction temperatures; the dynamic shear rheometer was used to measure response at maximum and intermediate pavement temperatures; and the bending beam rheometer and the direct tension device were used to measure response at lowest pavement temperatures. The study also addressed the high-temperature stability of the asphalt rubbers as well as the aging characteristics of these binders as reflected by the Thin Film Oven Test (TFOT) and Pressure Aging Vessel (PAV) aging procedures.
The paper includes analysis of the effect of high-temperature storage on rheological response at high and intermediate temperatures, the effect of rubber on the properties used for grading using the new SHRP specifications, and an evaluation of the change in aging characteristics of the selected asphalts as a result of adding the CRM.
CRM Effect 415
Materials and Experiment Design
There are different types of raw materials and different processes for reduction of CRM. In this study the rubbers were all produced from whole passenger tires. One type of CRM was produced by ambient shredding (AS), a second was produced by cryogenic grinding (CG), and a third was produced by a special extrusion process with the use of some additives (TP). The CRM's were selected to represent the materials that have the potential for dominating the paving market for CRM. The three rubbers were similar in size distribution and had a maximum particle size of approximately 1 mm. Four asphalts selected to cover a wide range in compositional properties were used. The asphalts varied in their asphaltene content, aromatic content, average molecular weight, and in their rheological and failure properties. Table 1 lists the chemical and physical characteristics of the asphalts. The asphalts included two AC-10 grade asphalts, an AR-2000, and a 200/300 pen. asphalt. No additives were used in producing the asphalt rubbers.
Table 1 Properties of Selected Asphalts Asphalt Type
A B C D
Grade 200/300 AR-2000 AC-10 AC-10
SHRP PG: 46-34 58-16 58-16 58-22
%Asphaltenes 16.2 5 13 4.8
%P. Aromatics 36 51 38.7 50
%N. Aromatics 36.1 35.3 34.6 41.3
%Saturates 11.4 6.6 11.9 3
Mixing was done using a high-speed lab mixer equiped with a heat mantle. Mixing was done in one-quarter gallon (3.8 liter) containers maintained at 160 ± 5C for one hour. The rubber to total mix was kept at 15 percent by weight of total mix for all rubber-asphalt combinations.
Testing was divided into four main parts:
Rotational Viscosity. This part had two objectives: First, to evaluate the change in consistency of binders after mixing the different rubbers; second, to evaluate the storage stability of the AR's. A Brookfield viscometer was used to test each AR at 135, 160, and 185C. The storage stability was evaluated after storage at only one temperature, 160C. Intermittent mixing was done during the storage period of 23 hours starting after the one hour of mixing.
Dynamic Shear Rheometry. As a result of SHRP research two parameters (G* and sin*) were selected to describe the rheological behavior of binders. The objective of this part was to measure the effect of CRM on these two parameters within the range of maximum and intermediate pavement temperatures. The measurements were done in a range of temperatures from 5 to 75C. These temperatures include the temperature ranges used in the current SHRP binder specification.
Flexural Creep and Failure Properties. At low pavement temperatures, SHRP requirements involve using the bending beam rheometer and the direct tension test for evaluating creep and direct-tension characteristics. This part of the study included measuring both responses at several temperatures to evaluate the influence of rubbers on asphalt properties.
Aging Characteristics. The TFOT and the PAV were used to investigate the aging behavior of asphalt rubbers and to compare it with the behavior of the base asphalts. For the evaluation, the dynamic shear rheometer, the
Bahia and Davies416
Figure 1 Relative Change in Rotational Viscosity at High Temperature
bending beam rheometer, and the direct tension test were used to measure properties before and after aging. The PAV aging was done at 100C to simulate moderate climate.
Results and Discussions
Consistency at High Temperatures Although not a property that affects pavement performance directly, consistency at high temperatures is
important to ensure that the binder can be pumped and mixed with aggregates, and that the total mix can be put down and compacted properly. SHRP specifications require that the viscosity at 135C is less than 3 Pa-s. The lower the viscosity, the better is the pumpability and constructability of the binder.
All CRM's, because of their particulate nature and high melting points, are expected to increase the viscosity of the base binder. This increase is, in fact, one of the most commonly reported disadvantages of asphalt rubbers. In addition, several studies have indicated that because of the interaction between asphalt cements and rubbers, a swelling-reaction phenomenon takes place and results in an unacceptable increase in viscosity (6). Asphalt-rubber producers use different approaches to control this phenomenon and produce an acceptable mix. It is well known that this phenomenon is both temperature-and time-dependent, and that if the wrong combination is used, major problems may arise.
Figure 1 depicts the relative increase in viscosities at 135 and 160C for two of the asphalts mixed with the three CRM's. The bar sets on the right represent the measurements after one hour of mixing, while the sets on the left represent the measurements after 23 hours of storage at